- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Annual Issues ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents
Journal of Chemistry
Volume 2013 (2013), Article ID 952954, 5 pages
Fast Microwave-Assisted Synthesis and Photoluminescence of CaWO4 Nanocrystals
College of Chemistry, Key Lab of Environment Friendly Chemistry and Application of Ministry of Education, Xiangtan University, Xiangtan 411105, China
Received 30 May 2013; Accepted 20 September 2013
Academic Editor: Jun Zhang
Copyright © 2013 Quanguo Li et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
In this work, CaWO4 nanoparticles have been synthesized by microwave-assisted method at a low temperature of 120°C. The as-prepared powders were characterized by X-ray powder diffraction (XRD), transmission electron microscopy (TEM), and Fourier transform infrared spectroscopy (FT-IR). It is found that the reaction time played an important role in the morphology controlling and crystallinity level of CaWO4 crystals. The effects of photoluminescent properties have a great relationship with crystallinity.
In recent years, with the advance of nanoscale materials science and technology, the synthesis of nanoscale materials with unique properties is becoming more and more important for studying the variation of materials’ properties with size and morphology [1–5]. Nanomaterials based on the scheelite-type have attracted considerable interest because of their luminescent property approved use in electrooptic applications [6–8]. SrWO4, CaWO4, PbWO4, and BaWO4 were considered to be typical oxides structure of scheelite-type. Locating within tetrahedral O-ion cages, W ions are isolated from each other in the scheelite structure, while Ca, Ba, Sr, and Pb ions are surrounded by eight oxygen ions .
CaWO4 with a scheelite structure is an important optical material, which has attracted particular interest because of its applications  in quantum electronics or scintillators as laser host material [11, 12]. CaWO4 powders are usually prepared by traditional solid-state reactions which require high temperature and harsh reaction conditions . Recently, CaWO4 nanoparticles have been prepared by various wet chemical methods [14–18], which needs long reaction time, or nonaqueous solvents, such as hydrothermal method, citrate complex method, combustion process, coprecipitation, microwave-hydrothermal methods, polymeric precursor method, and microwave-solvothermal methods [19–22]. Therefore, to synthesize CaWO4 nanoparticles with a mild method (e.g., low temperature and/or quick reaction time) is of significance in both fundamental and applied studies .
In this paper, we report the synthesis, crystal structure, and fluorescence property of CaWO4 nanocrystals, which is prepared from the reaction of CaCl2 and Na2WO42H2O in the presence of PEG1000 by fast microwave-assisted method. By controlling the different reaction time, the degree of crystallinity of CaWO4 can be controlled. It means that we can obtain CaWO4 with higher crystallinity target structure by adjusting the reaction time, which is important for the preparation of aimed productions in the system of Ca–W–O.
2. Experimental Section
CaCl2 (AR), Na2WO42H2O (AR), and PEG1000 (AR) were used as the starting materials, and all of them were of analytical grade without any further purification. CaWO4 nanocrystals were prepared by microwave-assisted method in the absence of any organic additives. In a typical procedure, 0.1093 g CaCl2 0.1003 g Na2WO42H2O, and 0.1409 g PEG1000 were put into quartz tube and dissolved in 10 mL distilled water, and the mixture was vigorously stirred for 10 min to ensure that all reagents were dispersed homogeneously. And then put the sealed quartz tube into the microwave reactor. Reaction temperature and time, pressure, and microwave power output were adjusted according to the parameters of the reactor. After cooling to room temperature naturally, the precipitates were collected, washed with distilled water and absolute ethanol for several times, and then dried in a vacuum oven at about 60°C for 24 h.
The morphologies of CaWO4 samples were examined by transmission electron microscopy (TEM) (JEM-2010, JEOL, Japan). The FT-IR spectra (Nicolet-380, Nicolet Instrument Co., USA) were recorded in the region of 4000–400 cm−1. X-ray diffraction (XRD) patterns were measured on a MiniFlex2 goniometer. Employing a scanning rate of 0.02°s−1 in the 2θ range from 5° to 70°, the operating voltage and current were maintained at 30 kV and 15 mA, respectively. Photoluminescence (PL) spectra were recorded by a Hitachi 850 fluorescence spectrometer with a Xe lamp at room temperature. Fourier transform infrared spectroscopic (FT-IR) analysis was carried out using pressed KBr disks in the region of 4000–400 cm−1 by using a Perkin Elmer spectrometer instrument.
3. Results and Discussion
3.1. Structural Analysis
The phase identification of all the products was performed by XRD. To investigate the effect of reaction time on the crystallinity, CaWO4 was prepared with different reaction time. The products synthesized at 120 degrees in 5 min, 10 min, and 15 min show similar patterns, which are in good agreement with the standard values for the tetragonal phase CaWO4 (Fm3hm, JCPDS No. 41-1431). Figure 1 shows the XRD patterns of the products obtained via microwave-assisted method. When reaction time is 5 min, the crystallinity of as-prepared product is considerably low, and there are few peaks that cannot be observed. Therefore, a longer time supports the formation of the thermodynamically stable, well-crystallized, and uniform products. It is very clear that the crystallinity of obtained products increase with the increasing of reaction time for 15 min (Figure 1(a)). In a word, the reaction time of the reaction systems was found to play an important role in determining the crystallinity of the CaWO4 nanocrystals.
To further confirm the formation of the CaWO4 crystal structure, Fourier transform infrared (FT-IR) spectroscopy was performed on the as-prepared CaWO4 nanocrystals (Figure 2). The bands at 1383 cm−1, 1576 cm−1, 1636 cm−1, and 3441 cm−1 are assigned to O–H stretching vibration and H–O–H bending vibration , respectively. The two bands are the characteristic vibrations of water from air absorbed on the sample surface physically which is completely different from coordinated water in compounds. The 111 cm−1 band is the characteristic vibrations of CO2 in the air. A strong absorption band around 800 cm−1 is related to O–W–O stretches of the WO4 tetrahedron, because the AWO4-type sheelite oxides, having S4 site symmetry for the WO4 groups, which show the main absorption bands in the region of 400–1000 cm−1, centered around 911, 405, and 833 cm−1 based on the v1, v2, and v3 modes of the WO4 groups, respectively . The 453 cm−1 band is attributed to the v2 stretching vibration of W–O on the same grounds.
3.2. Morphology Control
Figure 3 shows the typical TEM images of CaWO4 samples synthesized via microwave-assisted method at 120°C with different reaction time. It is very remarkable that CaWO4 nanocrystals are 63 nm in diameter, when reaction time is 15 min (Figure 3(c)). But the diameter of as-prepared CaWO4 is 46 nm and 62 nm, when reaction time is 5 min and 10 min (Figures 3(a) and 3(b)), respectively, which are in good agreement with the XRD results. This result further confirms that longer heating time would promote the crystallization of CaWO4 nanocrystals. Figure 3(c) shows that the spacing of the lattice fringe is 0.4835 nm and in consonance with the (101) face. Thus, it indicates that CaWO4 nanocrystals were synthesized by directional connection and self-assembly.
At room temperature, PL property of the CaWO4 nanoparticles was initially studied. Figure 4 shows the representative PL spectrum of the CaWO4 nanoparticles synthesized at 120°C for 5 min (a), 10 min (b), and 15 min (c), respectively. With the excited wavelength at 250 nm, the corresponding broad emission peak at 420 nm was observed. Further studies on PL property of the as-prepared CaWO4 nanoparticles were in progress. With the increasing of the reaction time, the emission peak value increases constantly, which has the same change with morphology and crystallinity. These results strongly indicate that the PL properties of CaWO4 are sensitive to the degree of structural order-disorder (crystallinity) and the relatively weak variations in the atomic arrangements which was basically in agreement with the analysis of Orhan et al. . In general, the possible reasons are associated with the charge-transfer transitions within the [WO4]2− complexes [26–29] or due to the vacancies as [WO3]  and [CaO7] .
CaWO4 nanocrystals have been successfully prepared by microwave-assisted method at a low reaction temperature of 120°C with different time. Experimental results indicated that the crystallinity of as-synthesized CaWO4 was affected by the reaction time. With the prolonging of the reaction time, the crystallinity of the sample got higher, and the average diameter of particles got bigger. The CaWO4 nanocrystal obtained by this preparation method has favourable luminance, which receives emissive wavelength at 420 nm with the excitation wavelength at 250 nm. It indicated that the kernel became bigger, the crystallinity was higher, and the intensity of fluorescence changed to become stronger as time went on.
The authors acknowledge with thanks the financial support of Provincial Natural Science Foundation of Hunan, China, (13JJ6041) and the National Natural Science Foundation of China (21343008).
Conflict of Interests
The authors declared that they have no conflict of interests to this work.
- Y. Wang, J. Ma, J. Tao et al., “Synthesis of CaWO4 nanoparticles by a molten salt method,” Materials Letters, vol. 60, no. 2, pp. 291–293, 2006.
- Y. Cui, Q. Wei, H. Park, and C. M. Lieber, “Nanowire nanosensors for highly sensitive and selective detection of biological and chemical species,” Science, vol. 293, no. 5533, pp. 1289–1292, 2001.
- M. H. Huang, S. Mao, H. Feick et al., “Room-temperature ultraviolet nanowire nanolasers,” Science, vol. 292, no. 5523, pp. 1897–1899, 2001.
- J. Hu, T. W. Odom, and C. M. Lieber, “Chemistry and physics in one dimension: synthesis and properties of nanowires and nanotubes,” Accounts of Chemical Research, vol. 32, no. 5, pp. 435–445, 1999.
- H.-W. Liao, Y.-F. Wang, X.-M. Liu, Y.-D. Li, and Y.-T. Qian, “Hydrothermal preparation and characterization of luminescent CdWO4 nanorods,” Chemistry of Materials, vol. 12, no. 10, pp. 2819–2821, 2000.
- G. Blasse and W. J. Schipper, “Low-temperature photoluminescence of strontium and barium tungstate,” Physica Status Solidi (A), vol. 25, pp. K163–K165, 1974.
- M. Martini, F. Meinardi, G. Spinolo, A. Vedda, M. Nikl, and Y. Usuki, “Shallow traps in PbWO4 studied by wavelength-resolved thermally stimulated luminescence,” Physical Review B, vol. 60, no. 7, pp. 4653–4658, 1999.
- M. A. M. A. Maurera, A. G. Souza, L. E. B. Soledade et al., “Microstructural and optical characterization of CaWO4 and SrWO4 thin films prepared by a chemical solution method,” Materials Letters, vol. 58, no. 5, pp. 727–732, 2004.
- M. Itoh and M. Fujita, “Optical properties of scheelite and raspite PbWO4 crystals,” Physical Review B, vol. 62, no. 19, pp. 12825–12830, 2000.
- M. J. Treadaway and R. C. Powell, “Energy transfer in samarium-doped calcium tungstate crystals,” Physical Review B, vol. 11, no. 2, pp. 862–874, 1975.
- S. Oishi and M. Hirao, “Growth of CaWO4 whiskers from KCl flux,” Journal of Materials Science Letters, vol. 8, no. 12, pp. 1397–1398, 1989.
- M. Kobayashi, M. Ishii, Y. Usuki, and H. Yahagi, “Scintillation characteristics of PbWO4 single crystals at room temperature,” Nuclear Instruments and Methods in Physics Research A, vol. 333, no. 2-3, pp. 429–433, 1993.
- G. Blasse and L. H. Brixner, “Ultraviolet emission from ABO4-type niobates, tantalates and tungstates,” Chemical Physics Letters, vol. 173, no. 5-6, pp. 409–411, 1990.
- M. Sadegh, A. Badiei, A. Abbasi, H. Goldooz, and G. Mohammadi Ziarani, “Preparation of CaWO4:Ln3+@SiO2 (Ln=Tb, Dy and Ho) nanoparticles by a combustion reaction and their optical properties,” Journal of Luminescence, vol. 130, no. 11, pp. 2072–2075, 2010.
- J. H. Ryu, J.-W. Yoon, C. S. Lim, W.-C. Oh, and K. B. Shim, “Microwave-assisted synthesis of nanocrystalline MWO4 (M: Ca, Ni) via water-based citrate complex precursor,” Ceramics International, vol. 31, no. 6, pp. 883–888, 2005.
- Q. Xiao, Q. Zhou, and M. Li, “Synthesis and photoluminescence properties of Sm3+-doped CaWO4 nanoparticles,” Journal of Luminescence, vol. 130, no. 6, pp. 1092–1094, 2010.
- J. k. Liu, Q. S. Wu, and Y. P. Ding, “Morphologies-controlled synthesis of CaWO4 crystals by a novel supramolecular template method,” Journal of Crystal Growth, vol. 279, no. 3-4, pp. 410–414, 2005.
- E. F. Paski and M. W. Blades, “Analysis of inorganic powders by time-wavelength resolved luminescence spectroscopy,” Analytical Chemistry, vol. 60, no. 11, pp. 1224–1230, 1988.
- L. Gracia, V. M. Longo, L. S. Cavalcante et al., “Presence of excited electronic state in CaWO4 crystals provoked by a tetrahedral distortion: an experimental and theoretical investigation,” Journal of Applied Physics, vol. 110, no. 4, Article ID 043501, 2011.
- V. M. Longo, L. Gracia, D. G. Stroppa et al., “A joint experimental and theoretical study on the nanomorphology of CaWO4 crystals,” Journal of Physical Chemistry C, vol. 115, no. 41, pp. 20113–20119, 2011.
- E. Orhan, M. Anicete-Santos, M. A. M. A. Maurera et al., “Towards an insight on the photoluminescence of disordered CaWO4 from a joint experimental and theoretical analysis,” Journal of Solid State Chemistry, vol. 178, no. 4, pp. 1284–1291, 2005.
- L. S. Cavalcante, V. M. Longo, J. C. Sczancoski et al., “Electronic structure, growth mechanism and photoluminescence of CaWO4 crystals,” CrystEngComm, vol. 14, no. 3, pp. 853–868, 2012.
- Y. Wang, J. Ma, J. Tao et al., “Synthesis of CaWO4 nanoparticles by a molten salt method,” Materials Letters, vol. 60, no. 2, pp. 291–293, 2006.
- A. Kato, S. Oishi, T. Shishido, M. Yamazaki, and S. Iida, “Evaluation of stoichiometric rare-earth molybdate and tungstate compounds as laser materials,” Journal of Physics and Chemistry of Solids, vol. 66, no. 11, pp. 2079–2081, 2005.
- F. Lei and B. Yan, “Hydrothermal synthesis and luminescence of CaMO4:RE3+ (M=W, Mo; RE=Eu, Tb) submicro-phosphors,” Journal of Solid State Chemistry, vol. 181, no. 4, pp. 855–862, 2008.
- D. Chen, G. Shen, K. Tang, H. Zheng, and Y. Qian, “Low-temperature synthesis of metal tungstates nanocrystallites in ethylene glycol,” Materials Research Bulletin, vol. 38, no. 14, pp. 1783–1789, 2003.
- S.-J. Chen, J. Li, X.-T. Chen, J.-M. Hong, Z. Xue, and X.-Z. You, “Solvothermal synthesis and characterization of crystalline CaWO4 nanoparticles,” Journal of Crystal Growth, vol. 253, no. 1–4, pp. 361–365, 2003.
- R. Zhai, H. Wang, H. Yan, and M. Yoshimura, “Preparation of crystalline CaWO4 thin films by chemical bath deposition,” Journal of Crystal Growth, vol. 289, no. 2, pp. 647–651, 2006.
- Z. L. Wang, G. Z. Li, and Z. W. Quan, “Nanostructured CaWO4, CaWO4/:Pb2+ and CaWO4:Tb3+ particles: polyol-mediated synthesis and luminescent properties,” Journal of Nanoscience and Nanotechnology, vol. 7, pp. 602–609, 2007.
- T. Liu, J. Chen, and F. Yan, “Optical polarized properties related to the oxygen vacancy in the CaMoO4 crystal,” Journal of Luminescence, vol. 129, no. 2, pp. 101–104, 2009.
- A. B. Campos, A. Z. Simões, E. Longo et al., “Mechanisms behind blue, green, and red photoluminescence emissions in CaWO4 and CaMoO4 powders,” Applied Physics Letters, vol. 91, no. 5, Article ID 051923, 2007.